advertisement

Chapter Outline: Phase Transformations Heat Treatment (time and temperature) ⇒ Microstructure ¾ Kinetics of phase transformations ¾ Homogeneous and heterogeneous nucleation ¾ Growth, rate of the phase transformation ¾ Metastable and equilibrium states ¾ Phase transformations in Fe-C alloys ¾ Isothermal Transformation Diagrams Not tested: in 10.5 Bainite, Spheroidite, Martensite… (from p. 360) 10.6 Continuous Cooling Transformation Diagrams 10.7-10.9 Mechanical behavior of Fe-C alloys, Tempered Martensite MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 1 Phase transformations. Kinetics. Phase transformations (change of the microstructure) can be divided into three categories: ¾ Diffusion-dependent with no change in phase composition or number of phases present (e.g. melting, solidification of pure metal, allotropic transformations, recrystallization, etc.) ¾ Diffusion-dependent with changes in phase compositions and/or number of phases (e.g. eutectic or eutectoid transformations) ¾ Diffusionless phase transformation - by cooperative small displacements of all atoms in structure, e.g. martensitic transformation (discussed in this chapter but not tested) Phase transformations do not occur instantaneously. Diffusion-dependent phase transformations can be rather slow and the final structure often depend on the rate of cooling/heating. We need to consider the time dependence or kinetics of the phase transformations. MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 2 Kinetics of phase transformations Phase transformations involve change in structure and (for multi-phase systems) composition ⇒ rearrangement and redistribution of atoms via diffusion is required. The process of phase transformation involves: ¾ Nucleation of the new phase(s) - formation of stable small particles (nuclei) of the new phase(s). Nuclei are often formed at grain boundaries and other defects. ¾ Growth of the new phase(s) at the expense of the original phase(s). S-shape curve: percent of material transformed vs. the logarithm of time. MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 3 Nucleation Nucleation can be Heterogeneous – the new phase appears on the walls of the container, at impurity particles, etc. Homogeneous – solid nuclei spontaneously appear within the undercooled phase. Let’s consider solidification of a liquid phase undercooled below the melting temperature as a simple example of a phase transformation. supercooled liquid liquid liquid solid homogeneous nucleation MSE 2090: Introduction to Materials Science solid heterogeneous nucleation Chapter 10, Phase Transformations 4 Gibbs free energy in analysis of phase transitions It is convenient to analyze phase transformations occurring under conditions of constant temperature (T) and pressure (P) by using Gibbs free energy (G). G = H – TS, where H is the enthalpy and S is the entropy H = U + PV, where U is the internal energy The conclusion of the thermodynamic analysis (take MSE 3050 to learn about the details) is that the equilibrium under conditions of T = const, and P = const corresponds to the minimum of G and a phase transformation occurs spontaneously only when G decreases in the course of the transformation Gibbs free energy (G = H – TS): Equilibrium is trade-off between minimization of enthalpy and maximization of entropy A change to a lower enthalpy state (ΔH < 0) usually decreases the randomness (ΔS < 0): MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 5 Homogeneous nucleation 1 2 supercooled liquid liquid solid Is the transition from undercooled liquid to a solid spherical particle in the liquid a spontaneous one? That is, is the Gibbs free energy decreases? The formation of a solid nucleus leads to a Gibbs free energy change of ΔG = G2 - G1 = -VS (GvL – GvS) + ASLγSL negative below Tm VS is the volume of the solid sphere ASL is the solid/liquid interfacial area always positive γSL is the solid/liquid interfacial energy ΔGv = GvL – GvS is the volume free energy difference at T < Tm, GvS < GvL – solid is the equilibrium phase MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 6 Homogeneous nucleation ΔG = G2 - G1 = -VS Δ Gv + ASLγSL 4 VS = π r 3 3 A SL = 4π r 2 For a spherical nucleus with radius r: 4 ΔG = - π r 3 ΔG v + 4π r 2 γ SL 3 interfacial energy ~ r2 ΔG ΔG * r* ΔG r volume energy ~ r3 For nucleus with a radius r > r*, the Gibbs free energy will decrease if the nucleus grows. r* is the critical nucleus size. MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 7 Homogeneous nucleation dΔ G At r = r* r* = = -4 π r 2 ΔG dr SL 2γ ΔG v + 8π r γ SL = 0 ( ) SL 3 16π γ ΔG = 2 3(ΔG v ) * v The difference between the Gibbs free energy of liquid and solid (also called “driving force” for the phase transformation) is proportional to the undercooling below the melting temperature, ΔT = Tm – T: ΔH m ΔT ΔG v = Tm where Hm is the latent heat of melting (or fusion) Therefore: ΔG SL ⎛ 2 γ Tm * ⎜ r =⎜ ⎝ ΔH m * ( ( ⎞ 1 ⎟⎟ ⎠ ΔT ) ⎛ 16 π γ SL 3 T 2 m =⎜ ⎜ 3 ΔH 2 m ⎝ ) ⎞ 1 ⎟ ⎟ (ΔT )2 ⎠ Both r* and G* decrease with increasing undercooling MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 8 Homogeneous nucleation ΔG ΔG ΔG 1* * 2 r2* r1* ΔG T2 < T1 < Tm ⎛ 2 γ SL Tm r = ⎜⎜ ⎝ ΔH m ⎞ 1 ⎟⎟ ⎠ ΔT ( ( ) * ΔG * ⎛ 16 π γ SL 3 T 2 m =⎜ ⎜ 3 ΔH 2 m ⎝ ) r ⎞ 1 ⎟ ⎟ (ΔT )2 ⎠ Both r* and G* decrease with increasing undercooling MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 9 Homogeneous nucleation There is an energy barrier of ΔG* for formation of a solid nucleus of critical size r*. The probability of energy fluctuation of size ΔG* is given by the Arrhenius equation and the rate of homogeneous nucleation is * ⎞ ⎛ ΔG & ⎟⎟ N ~ ν d exp ⎜⎜ − kT ⎠ ⎝ nuclei per m3 per s where νd is the frequency with which atoms from liquid attach to the solid nucleus. The rearrangement of atoms needed for joining the solid nucleus follow the same temperature dependence as the diffusion coefficient: ⎛ Qd ⎞ ν d ~ exp ⎜ − ⎟ ⎝ kT ⎠ Therefore: * ⎛ ⎞ Q ΔG ⎞ ⎛ d & ⎟⎟ N ~ exp ⎜ − ⎟ exp ⎜⎜ − kT ⎠ ⎝ kT ⎠ ⎝ MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 10 Rate of homogeneous nucleation * ⎛ ⎞ Q ΔG ⎛ ⎞ d & ⎜ ⎟⎟ N ~ exp ⎜ − ⎟ exp ⎜ − kT ⎠ ⎝ kT ⎠ ⎝ ⎛ Qd ⎞ exp ⎜ − ⎟ ⎝ kT ⎠ ⎛ ΔG * ⎞ ⎟⎟ exp ⎜⎜ − kT ⎠ ⎝ N& Tm Temperature ΔG* > Qd ( ) exp − ΔG* kT << exp(− Qd kT) ΔG* is too high - nucleation is suppressed ΔG* ≤ Qd ( ) exp − ΔG* kT > exp(− Qd kT) ΔG*~ 1/ΔT2 – decreases with T – sharp rise of homogeneous nucleation (diffusion is still active) exp(− Qd kT) – too small – low atomic mobility suppresses the nucleation rate MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 11 Heterogeneous nucleation liquid supercooled liquid solid the new phase appears on the walls of the container, at impurity particles, grain boundaries, etc. Let’s consider a simple example of heterogeneous nucleation of a nucleus of the shape of a spherical cap on a wall of a container. Three surface energies: γLC – liquid container interface, γLS – liquid-solid interface, γSC – solid-container interface. liquid γLC solid nucleus θ γLS γSC Balancing the interfacial tensions in the plane of the container wall gives γLC = γSC + γLS cos(θ) and the wetting angle θ is defined by cos(θ) = (γLC - γSC)/ γLS MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 12 Heterogeneous nucleation The formation of the nucleus leads to a Gibbs free energy change of ΔG = -VS ΔGv + ASLγSL + ASCγSC - ASCγLC One can show that ΔG het r ⎧ 4 = ⎨ - π r 3 ΔG ⎩ 3 v ⎫ + 4π r 2 γ SL ⎬ S (θ ) = ΔG ⎭ hom r S (θ ) where S (θ ) = (2 + cos θ )(1 − cos θ )2 /4 ≤ 1 ( dΔ G r = - 4π r 2 ΔG dr At r = r* 2 γ SL r = ΔG v * ΔG* v ) + 8π r γ SL S (θ ) = 0 ( ) 3 ΔG * het 16 π γ SL = S (θ ) = S (θ )ΔG 2 3 (ΔG v ) * hom ΔG *het ΔG * hom Active nucleation starts ΔT MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 13 Heterogeneous nucleation 2 γ SL r = ΔG v * if θ = 10 o ΔG * het = S (θ )ΔG * hom S (θ ) = (2 + cos θ )(1 − cos θ ) /4 ≈ 10 - 4 2 ΔG ΔG *hom ΔG *het r* nucleation rate heterogeneous nucleation starts at a lower undercooling heterogeneous homogeneous temperature MSE 2090: Introduction to Materials Science Tm Chapter 10, Phase Transformations 14 Growth Once a stable nucleus of the new phase exceeding the critical size r* is formed, it starts to grow. Atomically rough interfaces migrate by continuous growth, whereas atomically flat interfaces migrate by ledge formation and lateral growth. liquid liquid solid solid In multi-component systems, non-congruent phase transformations can involve long-range solute diffusion necessary for achieving the equilibrium phase composition. The atomic rearrangements necessary for growth of a onecomponent phase or growth in a congruent phase transformation, as well as the long-range diffusion of components in multi-component systems, involve thermally-activated elementary processes and can be described by Arrhenius equation: Growth rate = C exp (-QA/kT) = C exp (-Qm/ RT) per atom MSE 2090: Introduction to Materials Science per mole Chapter 10, Phase Transformations 15 Rate of phase transformations Total rate of a phase transformation induced by cooling is a product of the nucleation rate and growth rate (diffusion controlled - slows down with T decrease). overall transformation rate growth rate nucleation rate temperature Tm high T (close to Tm): low nucleation and high growth rates Æ coarse microstructure with large grains low T (strong undercooling): high nucleation and low growth rates Æ fine structure with small grains MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 16 Example of solidification under conditions of extreme undercooling Localized excitation of a metal film by a short laser pulse results in very steep temperature gradients, fast heat conduction and extreme cooling rates exceeding 1012 K/ s Æ deep undercooling of the melt Æ high nucleation rate Æ nanocrystalline structure of the surface feature generated by the laser pulse Ivanov, Lin, Rethfeld, O'Connor, Glynn, Zhigilei, J. Appl. Phys. 107, 013519, 2010 Atoms that belong to the fcc grains are colored blue, atoms with disordered local structure (liquid, grain boundaries, dislocations) are colored green. MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 17 Rate of phase transformations To quantitatively describe the rate of a phase transformation, it can be defined as reciprocal of time for transformation to proceed halfway to completion: rate = 1 / t0.5 Plotting the transformation time vs temperature results in a characteristic C-shaped curves: Tm temperature temperature Tm rate (1 / t0.5) log (t0.5) The analysis performed above for solidification can also be extended to other phase transformations, e.g. solid-state phase transformations. MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 18 Kinetics of phase transformations The time dependence of solid-state phase transformations at a fixed temperature is often described in terms of the time dependence of the fraction of transformation (y): S-shape curve: percent of material transformed vs. the logarithm of time. rate = 1 / t0.5 This time dependence of the fraction of transformation follows the Avrami equation: y = 1 – exp(-k tn) where k and n are time-independent constants for the particular transformation MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 19 Kinetics of phase transformations Temperature has a strong effect on the kinetics of the phase transformation and, therefore, on the rate of the phase transformation. Percent recrystallization of pure copper at different T: rate = 1 / t0.5 rate (135°C) >> rate (113°C) MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 20 Superheating / supercooling ¾ Upon crossing a phase boundary on the compositiontemperature phase diagram, phase transformation towards equilibrium state is induced. ¾ But the nucleation and growth of the equilibrium structure takes time and the transformation is delayed. ¾ During cooling, transformations occur at temperatures less than predicted by phase diagram: supercooling. ¾ During heating, transformations occur at temperatures greater than predicted by phase diagram: superheating. ¾ Degree of supercooling/superheating increases with rate of cooling/heating. ¾ Metastable states can be formed as a result of fast temperature change. Microstructure is strongly affected by the rate of cooling. ¾ Below we will consider the effect of time on phase transformations using iron-carbon alloy as an example. MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 21 Let us consider eutectoid reaction as an example eutectoid reaction: γ(0.76 wt% C) ↓ α (0.022 wt% C) + Fe3C The S-shaped curves are shifted to longer times at higher T showing that the transformation is dominated by nucleation (nucleation rate increases with supercooling) and not by diffusion (which tooccurs faster higher10,T). MSE 2090: Introduction Materials Scienceat Chapter Phase Transformations 22 Isothermal Transformation (or TTT) Diagrams (Temperature, Time, and % Transformation) MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 23 TTT Diagrams Austenite (stable) α ferrite Eutectoid temperature Coarse pearlite Fe3C Fine pearlite Austenite → pearlite transformation Denotes that a transformation is occurring The thickness of the ferrite and cementite layers in pearlite is ~ 8:1. The absolute layer thickness depends on the temperature of the transformation. The higher the temperature, the thicker the layers. MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 24 TTT Diagrams ¾ A family of S-shaped curves at different T are used to construct the TTT diagrams. ¾ The TTT diagrams are for the isothermal (constant T) transformations (material is cooled quickly to a given temperature before the transformation occurs, and then keep it at that temperature). ¾ At low temperatures, the transformation occurs sooner (it is controlled by the rate of nucleation) and grain growth (that is controlled by diffusion) is reduced. ¾ Slow diffusion at low temperatures leads to fine-grained microstructure with thin-layered structure of pearlite (fine pearlite). ¾ At higher temperatures, high diffusion rates allow for larger grain growth and formation of thick layered structure of pearlite (coarse pearlite). ¾ At compositions other than eutectoid, a proeutectoid phase (ferrite or cementite) coexist with pearlite. Additional curves for proeutectoid transformation must be included on TTT diagrams. MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 25 Summary Make sure you understand language and concepts: ¾ Avrami equation (for fraction of transformation) ¾ Coarse pearlite ¾ “Driving force” for phase transformation ¾ Fine pearlite ¾ Growth of a new phase ¾ Heterogeneous nucleation ¾ Homogeneous nucleation ¾ Isothermal transformation diagram ¾ Kinetics of phase transformations ¾ Nucleation barrier ¾ Phase transformation ¾ Rate of the phase transformation ¾ Size of the critical nucleus ¾ Supercooling ¾ Superheating ¾ Transformation rate MSE 2090: Introduction to Materials Science Chapter 10, Phase Transformations 26